Electro Optical Characterisation of Short Wavelength Semiconductor ...
Basic Concepts Semiconductor lasers have the smallest size, highest efficiency and longest lifetime of all the existing lasers. The fact of existence of many different applications for opto-electrical devices enabled the field of semiconductor lasers to draw the attention and resources necessary for its development. Optical communication was probably the first issue profited by this. The idea of optical storage media was the next great boom. Bar-code readers, laser printers and many military applications kept the topic an evergreen. All these commercially available laser diodes covered an emission spectrum from the red to the infrared. In order to be able to produce laser diodes emitting in green and blue other material systems were investigate. III-V nitrides such as gallium nitride, GaN, turned out to have a band gap in blue spectral region; II-VI selenides such as zinc selenide, ZnSe, in green. Although it was possible to manufacture light emitting devices, using deep luminescent centres, conducting p-type GaN was not obtained till 1988, when Akasaki and Amano accidentally discovered that the p-type dopant magnesium has to be activated . This happened by scanning electron microscopy investigation of the cathodoluminescence of Mg-doped GaN. Observations showed that the luminescence intensity increased with the scanning time . The passivity of Mg acceptors was later explained by the hydrogen atoms, which are released due to the energy of the electron beam. It took two more years until Nakamura developed an alternative activation technique. He removed the hydrogen by an annealing step in nitrogen . The first injection laser was presented in 1995 , six years after the first p-type doping. Today is Blu-ray Disc a strong motivation among others to push the whole business. The research on ZnSe-based laser devices was stimulated by the development of a reliable p-type doping technique in 1990 and 1991 [18, 19]. In the following years these devices were brought from short life pulsed operation at low temperatures (77 K) to continuous wave (cw) operation at room temperature. However with a limited life time due to which the ZnSe based lasers haven’t been commercialised yet and are still in research stage. 1.2 Physics of Semiconductor Lasers There are many different aspects needed to be observed by talking of semiconductor lasers. The building blocks of these structures are crystals. We also study the propagation of light in these crystal structures. Studying the crystals and the interaction of electromagnetic radiation and matter is therefore of importance. 1.2.1 Crystals An ideal crystal is built as the infinite repetition of identical structure units in the threedimensional space. In the simple crystals like copper, silver, iron, aluminium and the alkali metals the structure unit is only one atom. But in most of the cases there are different atoms or molecules which are contained in the crystal structure. Gallium nitride, zinc selenide and their related compounds can crystallise both in the zincblende as well as in the wurtzite structure. Crystallographically, the zincblende structure and wurtzite structure are very closely related. In a zincblende structure, a view along a  direction reveals that the atoms of a given kind are stacked in the sequence 4
Physics of Semiconductor Lasers · · · ABCABC · · · while maintaining tetrahedral bonds with those of the other kind. This diamond-like structure consists of two interpenetrating face-centred cubic bravais lattices, displaced along the body diagonal of the cubic cell by one quarter the length of the diagonal . The difference between a diamond and a zincblende structure is that a diamond has got an inversion centre in the middle of each connection line between two neighbours (Fig. 1.1) whereas the zincblende has no inversion symmetry (Fig. 1.2). In case of wurtzite structure the tetrahedral bond- Figure 1.1: Diamond structure  ing is preserved but the atoms of a given kind are stacked in the sequence · · · ABABAB · · · and the underlying Bravais lattice is hexagonal. Fig. 1.3 shows a clinographic projection of the wurtzite structure. In the clinographic projection the cube is turned through an angle θ about a vertical axis, making both the front and right hand faces visible. The cube is then projected on to a vertical plane by parallel straight lines, which are inclined to the horizontal so that the top face is brought into view . For the wurtzite structure the lattice constants a and b are equal which means a = b. The unit cell is described by c and a. The substructure of the unit cell creates an asymmetry of the unit cell along the c-axis, i.e the Figure 1.2: Zincblende structure  directions of the bonds are different along  and [000¯1]. It is worth adding that in case of hexagonal crystals the Bravais-Miller indices instead of Miller indices are commonly used. By Bravais-Miller figure the four indices (hkil) instead of the three (hkl) by Miller, whereas h + k + i = 0. The group-III nitrides are commonly found to grow in the hexagonal crystal structure, as this is the thermodynamically more stable modification. It is possible to obtain films showing a cubic lattice, but this requires the epitaxy on suitable cubic substrates. An interesting feature of the group III-nitrides is their exceptional hardness and chemical inertness combined with a good ther- Figure 1.3: Clinographic projection mal conductivity . This issue makes the group of the hexagonal wurtzite structure  III-nitride semiconductor devices stable, since high operation temperatures without destroying the lattice are possible. On the other hand 5
Appendix A Electrical Sources & Mea
ZnSe threshold current density valu
Bibliography  N. G. Basov, O. N.
BIBLIOGRAPHY  G. Snider, 1D Poi